## 2 Materials and Methods
\begin{table}
\begin{tabular}{c c c c c c} \hline \hline
**Group of Tape** & **Backing** & **Code** & **Thickness, \(\upmu\)m** &
\begin{tabular}{c} **Breaking Strength,** \\ **N/24 mm** \\ \end{tabular} & **Temperature Resistance \({}^{\ast}\)** \\ \hline \multirow{8}{*}{N} & \multirow{8}{*}{nonwoven} & N1 & 730 & 139 \(\pm\) 6.4 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & N2 & 840 & 80 \(\pm\) 5.0 & from \(-\)40 \({}^{\circ}\)C to +80 \({}^{\circ}\)C \\ \cline{3-6}  & & N3 & 780 & 96 \(\pm\) 2.7 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & N4 & 570 & 89 \(\pm\) 3.4 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & N5 & 570 & 90 \(\pm\) 7.1 & from \(-\)40 \({}^{\circ}\)C to +80 \({}^{\circ}\)C \\ \cline{3-6}  & & N6S & 630 & 120 \(\pm\) 4.2 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \hline \multirow{2}{*}{Pa} & \multirow{2}{*}{paper} & MPa1 & 370 & 107 \(\pm\) 10.8 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & Pa2 & 380 & 176 \(\pm\) 7.8 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & Pa3 & 450 & 144 \(\pm\) 10.0 & from \(-\)40 \({}^{\circ}\)C to +80 \({}^{\circ}\)C \\ \hline \multirow{4}{*}{P} & \multirow{4}{*}{films} & P1S & 390 & 33 \(\pm\)2.8 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & P2S & 370 & 53 \(\pm\) 4.8 & from \(-\)30 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & P3S & 380 & 35 \(\pm\) 2.7 & from \(-\)40 \({}^{\circ}\)C to +100 \({}^{\circ}\)C \\ \cline{3-6}  & & P4S & 360 & 45 \(\pm\) 3.3 & from \(-\)40 \({}^{\circ}\)C to +80 \({}^{\circ}\)C \\ \hline \hline \end{tabular}  
* S is reinforcement mesh, M is metalised paper;
* provided by the manufacturer.  
\end{table} 
Table 1: Summary of characteristics of self-adhesive tapes selected for investigation. Figure 2: Essential steps of the research process. Artificial aging is intended to simulate the effects of moisture, heat, and cold. The intensity, duration, and sequence of the cyclical effects of climatic factors were determined considering studies on the durability of the exterior layers of building walls [36]. This study was carried out after evaluating the statistical climatological data of the mid-latitude climate zone (air humidity, average duration of rain, number of sunny days, and changes in temperature in the warm and cold seasons). During an accelerated aging cycle, the test samples were heated for 7 h at +5 \({}^{\circ}\)C at a relative humidity of RH 96-100%, frozen for 5 h at \(-\)10 \({}^{\circ}\)C; 0.5 h of time was devoted to switching off the refrigeration. Realignment was followed by heating at different temperatures and humidity levels, i.e., they were heated for 18 h at +31 \({}^{\circ}\)C (RH = 45-50%), 10 h at +39 \({}^{\circ}\)C (RH = 25-30, %), and 7.5 h at +49 \({}^{\circ}\)C (RH = 15-20, %); the duration of the entire cycle was 48 h (Table 2). The artificial aging test was carried out in the Feutron 3423/16 climate chamber, with adjustable ambient conditions for temperature and humidity. The peel adhesion tests were performed after 1, 5, 10, 15, and 20 artificial aging cycles.